Crromics In~rnurroncrl23 ( 1996) 7 I I c 1996 Elsevier Saence Limited and Techna S.r.1. Printed m Great Britain. All rights reserved 0272-X842/97 $17.00 + 0.00
Titanium Disulphide Thin Film Prepared by Plasma-CVD for Lithium Secondary Battery Shinichi Kikkawa The Institute
of Scientific and Industrial (Received
24 July 1995; accepted
Osaka University. 29 August
Osaka 567, Japan
Abstract: Titanium disulphide fine power and preferred oriented thin film were prepared by plasma-CVD. The fine powder product was an aggregate of platelike crystallites of some IO nm in width, and less than IO nm in thickness. Crystalline orientation of TiS2 in the film was investigated in relation to deposition rate and film thickness. The preferred orientation of the TiS, basal plane perpendicular to the substrate was obtained on films with a thickness of more than _ IO pm at a deposition rate of -4x 10~ 3 g/cm’.h. Both the fine powder and the preferred orientation resulted in large discharge capacities in a lithium battery cathode application. 3’ 1996 Elsevier Science Limited and Techna S.r.1.
1 INTRODUCTION Applications of ceramic thin film have attracted increasing attention. It is very important to orient crystals in these films for the characteristics of the crystals to be emphasized. Plasma-CVD has been applied to prepare several kinds of high-tech ceramic materials. The method has been useful in obtaining thin film coatings and also fine powders of refractories. TiS2 is one of the most promising candidates for the lithium secondary battery cathode.’ Lithium ions are intercalated in the TiS2 crystal lattice forming Li,TiSz (OS&l). The reaction energy is released as electrical energy from the battery. The lithium ion has to diffuse in the TiS2 crystal lattice during the reaction. A large surface area is necessary to obtain a high current density. The Li intercalation occurs along the TiS2 layer, and it is difficult to intercalate Li+ from a direction perpendicular to the host layer. The battery charge and discharge occur with lithium intercalation and deintercalation. It seems to be very important that the very fine TiS2 powder orients its layer plane perpendicular to the lithium anode surface in order to enhance current density. In the discharging process, most of the lithium ions are electrostatically absorbed on the TiS2 film surface if TiS2 crystals orient their layer planes parallel to a substrate, as
schematically shown in Fig. l(a). If the crystals stand perpendicularly, as shown in Fig. l(b), the Li+ is easily intercalated to the TiS2 inter-layer space in an applied electric field. Chemical vapour deposition of titanium disulphide has been investigated in a classical way using an electrical furnace. The products formed in a quartz substrate were large TiS2 crystals (-2 100 urn thick) having relatively random orientation. It is not easy to obtain stoichiometric TiS2 due to the presence of the non-stoichiometric titanium-rich compositional range Ti, +_& and also the higher sulphide TiSs. The non-stoichiometry x of Ti, +.,Sz increases with an increase in firing temperature. TiS3 is obtained under high sulphur pressure and at lower temperature than the preparation conditions of TiS,.’ It is important to set up an optimum temperature and sulphur pressure to obtain stoichiometric TiS?. The chemical diffusion constant of sodium ion in TiS? was very much reduced with the non-stoichiometry. However, a recent investigation showed that the diffusion constant of Li’ was not much reduced, but the amount of the intercalated Li + decreased.’ A large amount of non-stoichiometry is unfavorable. but a trace amount may be permitted for the battery application. Application of plasmaCVD seems very useful in obtaining TiSz fine powder and its preferred oriented thin film.4mh
In the present investigation, a plasma-CVD reactor of parallel-plate type was used to obtain Ti& fine powder and its preferred oriented thin film. The products were characterized by X-ray diffraction, SEM, TEM, etc., and they were applied for the lithium secondary battery cathode.
2 EXPERIMENTAL A reaction vessel of lop2 m3 was evacuated and then TiC14 (99.9% pure) was supplied at a rate of 4.9x 10p5-1 .7x 10e3 mol/min, with Ar carrier at a flow rate of 10 cm3/min. H2S (99.9% pure) was introduced at a rate of 5-100 cm3/min. The reaction was performed by applying a high frequency (13.56 MHz) with an electric power of l&125 W for a duration of 2-60 min. Prior to the deposition, the substrates were etched with Ar for 30 min, with a substrate temperature (7’s) of 300°C and rf power of 50 W. The supply rate of Tic& was controlled by changing the temperature of the Tic& reservoir. The products were characterized by XRD, TEM and SEM. 1M LiC104-tetrahydrofuran (THF) was used as an electrolyte-solvent in the lithium battery. Discharge and charge were performed at a constant current of 0.15 mA/ cm2, in the range 2.7-1.5 V.
Fine black powder was obtained on a thin film deposited on a glass substrate. The powder portion of the total deposit (film and fine powder) was dependent both on the reaction pressure and on the deposition site on the lower electrode. The powder was obtained in high yield under a pressure of 120 Pa at the electrode centre, where the plasma density was high. Its deposition rate had a maximum value of N 5 x 10e3 g/cm2.h at the centre of the reactor electrode, and rapidly decreased along the radial direction. The following investigations were performed on the products obtained at the centre.
Substrate 0 (a) Fig. 1. Schematic
The variety of product phases characterized by XRD depended both on the magnitude of the rf power and also on the substrate temperature. Figure 2 depicts a formation diagram obtained at a reactant ratio of [H2S]/[TiCl,] z 3. TiS2 powder was obtained on thin films of TiS2 or of TiS2 contaminated with a small amount of TiS3 at reaction conditions represented by the circles and squares, respectively. At conditions depicted by the triangle and crosses, the powders were mixtures of TiS2 and TiS,. TiS2 had been prepared above 600°C by a classical method.2 TiS2 fine powder was obtained on a substrate heated up to 450 “C in the present plasma-assisted CVD. The preparation temperature for TiS2 was reduced with the application of plasma. The real composition of the TiS2 described above was a non-stoichiometric Tir +S2. TiS2 has a titanium-excess non-stoichiometric composition range, where the c-lattice parameter expands from 0.5695 nm with the increasing titanium content.’ The powder deposited at 450 “C and 12 W had the shortest c-parameter (0.584 nm) among the products in Fig. 2. Thermogravimetry showed its composition to be Tir.r&. 3.1 Ti& fine powder Stoichiometric TiS2 had been synthesized from the reaction of TiC14 + 2H2S-tTiS2 + 4HCl in a closed reaction system. A molar ratio of 2 for H2S to Tic& might be sufficient to attain a stoichiometry of TiS2. The present products had titanium-excess non-stoichiometry because H2S was removed faster than TiC14 from the reaction vessel during the continuous evacuation during the reaction. The H2S flow was increased under the most favorable
Substrate 0 Substrate temperature/T
(b) representation for the cathode Li/Ti& thin film battery.
Fig. 2. Formation
of titanium thin film.
Titanium disulphide thin ,$lm
conditions of 450°C and 12 W. The lattice parameter c continuously shrank with the increasing [H$]/[TiCl,] reactant ratio. The stoichiometric composition Ti1.0S2 with c =0.570 nm was attained in the powder product with a reactant ratio of 27. Titanium disulphide crystallizes in a hexagonal CdI,-type crystal lattice. Crystallite sizes of the fine powder were estimated from the broadening of the XRD(OO1) line to be about 5 nm, and a value of about 18 nm was obtained from the (110) line. X-ray diffraction peaks for T&S3 overlap with many of these for TiS*. However, the present product was not contaminated with Ti2S3 because the strongest 104 diffraction line of Ti& (JCPDS 35-l 135) was not observed. TEM observations showed an aggregation of plate-like crystallites of about 40 nm in width and about 10 nm in thickness, as shown in Fig. 3. Figure 4 shows the discharging behaviour of Lij 1M LiC104 in THF/Ti i +_SZ cells. A utilization of 100% corresponds to the discharged electricity necessary to obtain LiTi& by the Li intercalation into TiSZ. A rapid potential drop was observed for the cell using a coarse powder of Ti I.OOSZ prepared
Fig. 3. TEM photograph
of TiSz fine powder.
Ti I.!‘) s ? fine powder Li(IM
by the sealed-tube method before full utilization was attained. The Ti l.i&z fine powder cell could be discharged continuously to full utilization. It generated a slightly lower voltage than the Ti1.00S2cell described above. The voltage reduction is mainly attributed to its non-stoichiometry. The cell interior resistivities may not differ so much: lithium ionic diffusivity is not greatly affected by the nonstoichiometry.3 These cells were discharged at a current density of 0.5 mA/cm’. A relatively flat discharge curve was also observed for the cell using Til,oSz fine powder, in spite of a higher current density of 1.5 mA/cm 2. Its generated voltage was slightly lower than that of Ti1.00S2 due to the higher current density. The cell was cycled in voltage limits between 2.7 and 1.5 V. Its discharge capacity continuously decreased to -40% after the 50th dischargesharge cycle. 3.2 Preferred oriented TiS2 film The products were mainly films without contamination of powder when the deposition rate was slower than 7.5x 10-j g/cm’.h. The preferred orientation of the c-plane parallel to the substrate became stronger with a decrease of the deposition rate to 2.2x 10e4 g/cm’.h. Almost perfect preferred orientation was attained at a rate of 2.2x lop4 g/ cm’.h. Crystalline orientation also changed with the film thickness. Deposition rate was kept almost constant in the range 3.1-4.1 x IO-” g/cm’.h. A thin film of 2.3 urn thickness showed an intense 001 Xray diffraction line, as shown in Fig. 5. The 001 peak disappeared and an intense 110 line was observed for a film of 13.5 urn thickness. These results suggest that the TiS2 basal plane is parallel to the substrate in a thin film. With increasing film thickness, the TiSz layer gradually stands up, and it is perpendicular to the substrate in films which are > 10 ym thick. The surface texture of the 2.3 urn
13.5 pm IO0
Fig. 4. Discharge curves of Ti, + ,&/Li batteries. Full and dotted lines represent lithium battery discharges using fine powder prepared by plasma-CVD and coarse powder prepared by the classical method, respectively.
Fig. 5. X-ray
diffractograms of TiSr thin film with various film thicknesses.
Film surface thickness : 7.3 km
Film surface thickness : 2.3 p.m C(b)
Film surface thickness : 13.5 pm
Cross-section thickness : 13.5 pm
Fig. 6. SEM observation of surface and cross-sectional textures for TiS2 thin film with various film thicknesses. Discharge capacity 0
8 0.5 _..
0.15 mA/cm2 LI ( 1M LiC104-THF 1Ti,+&lStainless , I I I , t zo 40 60 80 100 120 Utilization
steel t 140 160
Fig. 7. Discharge curves for the lithium batteries using TiS2 thin film with different crystal orientation as the cathode.
thick thin film showed that plate-like crystals were deposited, keeping their basal plane parallel to the substrate, as depicted in Fig. 6(A). Flat basal planes were observed even in the coagulated particles with a diameter of 0.5 )_tm. The film surface had small homogeneous ridges on the film which were N 10 urn thick, as indicated in Fig. 6(B) and (C(a)). The plate-like TiS2 crystals stand perpendicularly to the substrate forming a columnar texture, as shown in the cross-sectional picture of Fig. 6(C(b)). T& crystallites easily grow in their (00 1) plane, which is their closest packing plane. In the beginning of the deposition process, mostly (001) plane-preferred oriented TiSz crystallites cover the whole substrate
surface. Once the TiS2 crystallites cover the whole substrate surface, a small portion of the crystallites (having a slight misorientation of (001) orientation from the substrate surface) grow continuously in their own (001) plane. With increasing film thickness, the ratio of TiSz (110) plane-preferred orientation gradually increases because the gas species are supplied along the direction perpendicular to the substrate. The easy growing direction of the crystal coincides with the gas supplying direction above. Lithium battery performance was studied on the TiS2 thin film prepared under various conditions. Figure 7 represents discharge curves for the batteries where the TiS2 film was deposited on stainless steel. One mole of TiS2 can reversibly intercalate one mole of Lif . A 100% utilization in the abscissa corresponds to the discharge capacity to obtain LiTi& The value of IIiO/ltotat tentatively represents the degree of preferred orientation. A larger discharge capacity was observed for the battery using TiS2 film with a high ZIlO/ltotai percentage. The film having a TiS2 crystal basal plane perpendicular to the substrate seems to show a large discharge capacity, probably because Li intercalation occurs easily when a Lit ion is supplied along the TiS2 basal plane, as shown in Fig. l(b). The films deposited on carbon substrate showed the same tendency as that observed for stainless steel. TiS2 crystalline orientation changed
Titanium disulphide thin film
100‘4 t Fig. 8.
with its deposition rate and also with the film thickness. The discharge capacity was correlated to TiSz crystallite orientation. Transmission electron micrography showed that T& prepared by plasma-CVD had a higher density of crystalline defects than that for TiS2 obtained by a reaction between Ti and S at high temperature. Figure 8 shows transmission electron micrographs of TiSz fine powder prepared by plasma-CVD in high magnification. The stripe lines corresponding to the TiS2 (001) plane are not straight, discontinuous or unclear anywhere. The distance between the iines is not uniform. There are many kinds of crystalline defects. The high density of these defects is a characteristic of plasma-CVD
in high magnification.
TiS2 and it may contribute to the unexpectedly large discharge capacity of the lithium battery.
M. S., Prog.
Solid State Chem., 12
(1978) 41 M. S & PANELLA. J. A., /Mater. 1. WWTTTINGHAM, Res. Bul(, 16 (1984) 37. 3. YAMAMOTO, T., KIKKAWA, S. & KOIZUMI, M.,
Solid Stale Ionics, 17 (1985) 63. 4.
R. S. & KOIZUMI,
Appl. Phys., A49 (1989) 105. 5.
M. & KOIZUMI,
Maier. Rus.. 5 (1990) 2894. 6.
KIKKAWA, S., MIYAZAKI, M., LIU, Y. & KANAMARLJ. F.. Solid Stutr Zonrcs, 40-41 (1990) 553.